Popular Non Destructive Testing of Concrete Structure
Download Popular Non Destructive Testing of Concrete Structure...
L O G IN
MA GA Z INE S
C R E A T E A N AC C O U N T
HOME ABOUT US CONTACT US
E QUIPME NT S
RE PORT S
INT E RVIE WS
PE OPLE WA T CH
Popular Non Destructive Testing of Concrete Structure-review of Std. Methods
R. B. Singh, Singh, Chief Coordinator, ANULAB, Agra Introduction View Online View Download Issue (PD (PDF) F) Previous Previ ous Issue s
View Vi ew Online Download Issue (PD (PDF) F) Previous Previ ous Issue s
A D V E R T I S E W IT H U S
In a short span of ten years after Bhuj earthquake, nondestructive testing has achieved an important place in the Quality Assurance of hardened concrete and the evaluation of existing concrete s tructure with regard to t heir strength & durab ility. ility. This paper deals with the popular, economical and widely used NDT tests in the field in general & national highways in particular. The paper also has discussion on combined methods, when more than one nondestructive test method is used and condition asse ssment is based on the da ta obtained from Rebound Hammer Hammer,, UPV & Core tests. The aim of the paper is to address the field engineers engaged in evaluation of quality of hardened concrete. An attempt has been made to keep the theoretical part of the subject to an absolute minimum, where necessary tables of std. values, photographs & comparisons have been included. Research oriented engineers who would want through treatment of the material and a more basic approach are referred to the original std. specification, NDT handbooks & original papers and literature on the subject given as reference. Although nondestructive tests are relatively simple to perform & instrument based, the analysis and interpretation of the test data are not easy, because concrete is a complex material, hence the engineers are cautioned that interpretation of the test data must always be carried out by trained specialists in NDT rather than by technicians performing the tests. If used properly, nondestructive tests can form a vital link in the chain of testing and evaluation of concrete and concrete structures, which starts with crushing of 150 mm cubes and may end with load testing of finished structure. At present, standard method of determination strength of hardened concrete consist of testing of concrete cubes (03 Nos. of 150X150X150 mm) in compression testing machine following the std. test method IS: 516. In case of PQC for rigid pavement, beam specimens are broken for flexural strength. The strength tests, regardless of the type, are excellent for determining the criteria of quality & quality control during construction, but they leave a lot to be desired. The main disadvantage of such tests are delay in obtaining test results, the fact that the test specimen may not be truly representative of the concrete in a structure, the necessity of stressing the test specimen to failure, the lack of reproducibility in the test results and the relativity high cost of testing & wastage of concrete in form of cubes.
E VE NT S
View Online Download Issue (PDF) Previous Issue s
For the NDT tests to monitor the service behavior of concrete structures over a long period, it was imperative that these tests be nondestructive. This approach, though new for the testing of concrete, had long been used in the testing of metals in petroleum exploration & refining projects. The direct determination of strength implies that concrete specimen must be loaded to failure; it becomes clear that nondestructive methods of testing cannot be expected to yield absolute value of strength. These methods, therefore, attempt to measure some other property of concrete from which an estimate on its strength, its durability and its elastic parameters is obtained. Such properties of concrete are its hardness, rebound number and its ability to allow ultrasonic pulse velocity to propagate through it. The electrical properties of the concrete, allow us to estimate its moisture content, density, thickness and its cement content. Based on above, various nondestructive methods of testing concrete have been developed. Pop ular NDT Tests for Concrete Use d in field are: 1. Rebound Hammer Test- RH Test 2. Ultrasonic Pulse Velocity- UPV Test 3. Combined Method UPV & RH Test 4. Core Extraction for Compressive Strength Test 5. Ingredient Analysis of Concrete Core 6. Concrete Cover Measurement by Laser Based Instt. This pa per, des cribes in detail only Rebo und Hammer (RH) test, Ultrasonic Pulse Velocity (UPV) test & Core Test which are widely used & accepted by engineers at site and also referred in IS: 456-2000, under Inspection & Testing of Structures. These are followed by a description of the combined methods approach in which more than one nondestructive method is used to estimate strength of concrete. The Ingredient Analysis, Cover Measurement, Permeability, and Density methods are of limited application and are briefly described the concluding part of the paper. 1. Rebound Hammer–RH (Schmidt) Test Currently O nline
In 1948, a Swiss Engineer, Ernst Schmidt from Zurich developed a test hammer for measuring the hardness of concrete by the rebound principle. Since then the Rebound Hammer (RH) tes t has g ained recog nition at con struction site & precas t Industry.
We have 168 guests online Alexa Rank
Principle The Schmidt Rebound Hammer is principally a surface hardness tester with little apparent theoretical relationship between the strength of concrete and the Rebound number of the hammer. However, within limits, empirical correlations have been established betw een s trength properties & rebound number. This correlation betw een the concrete strength and rebound number is required to be established at site/field laboratories before it is used for strength estimation of concrete. Sometimes it is referred as fieldcalibration of rebound hammer. Lab calibration are based on Brinell Hardness & Rebound Nos. are checked on std. calibrated Anvil for the purpose. Proper site calibrations eliminate the lab calibration, which is for the checking of hammer performance. Rebound Number and Compressive Strength There is a general correlation between compressive strength of concrete and the hammer rebound number. Coefficients of variation for compressive strength for a wide variety of specimens averaged 25%. The large deviations in strength can be narrowed down considerably by proper calibration of the hammer, which allows for various variables discussed earlier. By consensus, the accuracy of estimation of compressive strength of test specimens cast, cured, and tested under laboratory conditions by a properly calibrated hammer lies between ±15 and ±20%. However, the probable accuracy of prediction o f concrete streng th in a structure is ±25%. Limitations and Usefulness The limitations of the Schmidt hammer are many; these should be recognized and allowances be made when using the hammer. It cannot be overstressed that this instrument must not be regarded a s a substitute for standard compression tests b ut as a method for determining the uniformity of concrete in the structures and comparing one concrete by the Schmidt hammer within an accuracy of ±15 to ±20% may be possible only for specimens cast, cured, and tested under identical conditions as those from which the calibration curves are established. The prediction of strength of structural concrete by using calibration charts based on the laboratory test is not recommended.
2. Ultrasonic Pulse Velocity-UPV Test The test instrument consists of a means of producing and introducing a wave pulse into the concrete and a means of sensing the arrival of the pulse and accurately measuring the time taken by the pulse to travel through the concrete. Portable ultrasonic testing equipment are available. The equipment is portable, simple to operate, and includes rechargeable battery and charging unit. Typically, pulse times of up to 6500 os can be measured with 0.1-os resolution. The measured travel time is prominently displayed. The instrument comes with a set of two transducers, one each for transmitting and receiving the ultrasonic pulse. Transducers with frequencies of 25 to 100 KHz are usually used for testing concrete. These transducers primarily generate compressional waves at predominantly one frequency, with most of the wave energy directed along the axis normal to the transducer face. Factors Affecting UPV Test Although it is relatively easy to conduct a pulse velocity test, it is important that the test be conducted such that the pulse velocity readings are reproducible and that they are affected only by the properties of the concrete under test rather than by other factors. The factors affecting the pulse velocity can be divided into two categories: (1) factors res ulting directly from concrete prope rties; and (2) othe r factors. These influencing factors are discussed below: Effects of Concrete Properties 1. Aggregate Size, Grading, Type, and Content 2. Cement Type 3. Wa ter-Cement Ratio 4. Admixtures 5. Age of Concrete Other Effects 1. Transd ucer Conta ct 2. Temperature of Concrete 3. Moisture and Curing Condition of Concrete 4. Path Length 5. Size and Shape o f a Specimen 6. Level of Stress 7. Pres ence of Reinforcing Steel Applications of UPV Tests The pulse velocity method has been applied successfully in the laboratory as well as in the field. It can be used for quality control, as well as for the analysis of deterioration. The applications of the pulse velocity method on a concrete structure are: 1. Estimation of Strength of Concrete 2. Esta blishing Homogeneity of Concrete 3. Studies on the Hydration of Cement 4. Studies on Durability of Concrete
UPV Test being perform on Deck Slab of
5. Measure ment of Surface Crack Depth
Flyover on NH-2 at Firozabad (U.P.), India
6. Dete rminat ion of Dynamic Modu lus of Elas ticity Combined Method–UPV & RH Test Hardness scales are arbitrarily defined measures of the resistance of a material to indentation under static or dynamic load or resistance to scratch, abrasion, wear, cutting or drilling. Concrete test hammers evaluate surface hardness as a function of resiliency, i.e the ab ility of hammer to rebound o r spring back. The
measurements in concrete is complicated by the heterogeneous nature of this material. The wave velocity is not determined directly, but is calculated from the time taken by a pulse to travel a measured distance. A piezoelectric transducer emitting vibration at its fundamental frequency is placed in contact with the concrete surface so that the vibrations travel through the concrete and are received by another transducer, which is in contact with the opposite face of the test object. UPV Test being perform on Minor Bridge
Pier on NH-11 at Dausa (Raj.), India
Combined nondestructive methods refer to techniques in which one test is used to improve the reliability of the in site concrete strength estimated by means of another tes t alone. The validity of a combined technique can be evaluated from the degree of improvement this additional test provides to the accuracy and reproducibility of predictions, vs. the additional cost and complexity of the combined method and the extent to which it is practicable to perform the additional test in site. Portable Concrete Coring Machine
Of the various combinations proposed by (BOSCH) in Horizontal Operation on RCC different researchers and from the reported Column data it seems that only the combined techniques based on the Ultrasonic Pulse Velocity and surface ha rdness measurement have been adopted for practical evaluation of the in site compressive strength of concrete. The limitations of a combined method are usually those pertinent to the limitations of each component test, except when a variation in the properties of concrete affects the component test, except when a variation in the properties of concrete affects the component test results in opposite directions. In this case, the errors can be self-correcting. Development of a prior correlation relationship is essential if the estimated from the combined test are to be meanigful. The more information that can be Concrete Core from RCC Column be ing obtained about the concrete ingredients, Extracted after Diam ond Bit Core Drilling proportions, age, curing conditions, etc. the more reliable the est imate is likely to be. When testing suspect quality concrete of unknown composition, it is highly desirable to develop a prior correlation relationship in which factor such as aggregate type and approximate age of concrete are introduced as constants. For most in site concrete an approximate age and petrological type of aggregate can be determined, thus reducing the number of uncontrollable variables. The most important influences on the accuracy and reliability of strength estimates seem to be the coarse agg regate type in the concrete. When a reliable prior correlation relationship exists for a particular concrete type, the use of combined nondestructive techniques provides a realistic alternative to destructive testing. It often possible to perform a large and thus a representative number of tests at a reduced Core Drilling in Progress on the Inside cost compared with coring, and without an Wall (After Epoxy Grouting) of Box C ulvert adverse effects on the integrity of structural on NH-26 at Sagar, (M.P.) element. Core Extraction for Compressive Strength Test Test Specimens Core Specimens- A core specimen for the determination of compressive strength shall
have a diameter at least three times the maximum nominal size of the coarse aggregate used in the concrete, and in no case shall the diameter of the specimen be less than twice the maximum nominal size of the coarse aggregate. The length of the specimen, when capped, shall be as nearly as practicable twice its diameter. Procedure Core DrillingA core specimen taken perpendicular to a horizontal surface shall be located, when possible, with its axis perpendicular to the bed of the concrete as originally p laced.
Core Dressing-Cutting in Lab using Diamond Whe el Cutter in the Lab be fore Capping and C uring for Comp ressive Strength Test on CTM
Measurement of Drilled Core Specimens Mean Diameter- The mean diameter shall be determined to the nearest millimeter from three pairs of measurements. The two measurements in each pair shall be taken at right angles to e ach other, one pair being taken at the middle of the core and the o ther pairs at the quarter points of the depth. The mean of the six readings shall be taken as the diameter. Position of Reinforcement- The positions of any reinforcement shall be determined by measuring to the nearest millimetre from the centre of the exposed bars to the top of the core. The diameter and, if possible, the spacing of the bars shall be recorded, and also t he minimum top a nd bo ttom cover. Capping- The ends of the specimen shall be capped before testing. The material used for the capping shall be such that its compressive strength is greater than that of the concrete in the core. Caps shall be made as thin as practicable and shall not flow or fracture before the concrete fails w hen the specimen is te sted. The capped surfaces shall be at right angles to the axis of the specimen and shall not depart from a plane b y more than 0.05 mm. Apparatus Number of Specimens- At leas t three s pecimens, preferably from different batche s, shall be made for testing at e ach selected age.
Extracted Three Numbers of Cores (Making One Sample) from RCC Structure-Box Culvert on NH-26 at Sagar (M.P.)
Procedure- Specimens stored in water shall be tested immediately on removal from the water and while they are still in the wet condition. Surface water and grit shall be wiped off the spe cimens a nd any proje cting fins removed. Specimens whe n received dry shall be kept in water for 24 hours before they are taken for testing. The dimensions of the spe cimens to the nearest 0.2 mm and their weight shall be noted before testing. CalculationThe measured compressive strength of the specimen shall be calculated by dividing the maximum load applied to the specimen during the test by the cross-sectional area, calculated from the mean dimensions of the section and shall be expressed to the nearest kg per sq cm. Average of three values shall be taken as the representative of the batch provided the individual variation is not more than ± 15% of the average. Otherwise repeat tests shall be made. A correction factor according to the height/diameter ration of specimen after capping shall be obtained from the hardened curve. The product of this correction factor and the measured compressive strength shall be known as the corrected compressive strength, this being the equivalent strength of a cylinder having a height/diameter ratio of two. The equivalent cube strength of the concrete shall be determined by multiplying the corrected cylinder streng th by 5/4.
Cappe d and C ured Concrete Core Specimen under Compressive Strength Test in CTM
Report- The following information shall be included in the report on each test specimen/core: a. Identification Mark, b. Date of test, c. Age of Specimen, d. Curing Conditions, Including da te Manufacture of Specimen in the Field,
e. We ight of Specimen f. Dimens ions of Specimen, g. Cross -Sectional Area,
Cappe d and C ured Concrete Core Specimen under Compressive Strength
h. Maximum Loa d,
Test in CTM
i. Compress ive Strength, and
j. Appe ara nce of Fracture d Face s of Con crete and Type of Fracture , if the se are Unusual. Reference IS: 13311 (Part 1): 1992 Non-Destructive Testing of Concrete-Method of Test; Part 1-Ultrasonic Pulse Velocity. IS: 13311 (Part 2): 1992 Non-Destructive Testing of Concrete-Method of Test; Part 2-Reboun d Hammer. BS: 1881: Part 203: 1986 British Standard-Testing Concrete Part 203. Recommenda tions for Meas urement of Velocity of Ultrasonic Pulses in Concrete . ASTM C 597-02 Standa rd Test Method for P ulse Velocity through Co ncrete. Handbook on Nondestructive Testing of Concrete, Second Edition, Edited by V.M. Malhotra and N.J. Carino, ASTM & CRC Press , 2006. Testing Hardened Concrete: Nondestructive Methods by V.M. Malhotra, Published Jointly by the IOWA State University Press & American Concrete Institute (ACI) 1976. Near-Surface Testing for Strength and Durability of Concrete, Editor P.A.M. Bashee r, Fifth CANMET/ACI International Co nference o n Durability of Con crete. Advanced Testing Methods and Damage Assessment of Distressed Concrete Structures by H.G. Sreenath Proceedings of the Advanced Course on Structural Health Monitoring, Repair and Rehabilatation of Concrete Structures Feb. 4-6, 2006, SERC, CSIR, Chennai. Advanced Course on Non-Destructive Testing and Evaluation of Concrete Sructures, Orga nised by SERC, CSIR.Chenna i, 2006. Properties of Concrete, Fourth Edition 1996, by A.M. Neville, Published by ELBSLongman. Acknowledgement The article has been reproduced from the proceeding of "National Seminar on Green Structures for Susta inability" w ith the kind permission from the e vent orga nisers. NBMCW October 2010
< Prev T ERMS & CONDIT IONS
PRIVA CY POLICY
C A NC E LLA TION/ RE F UND POL IC Y
DIS C LA IME R
Copyright © 2010 NBM Media P vt. Ltd. All Rights Reserved.